1. Chapter 3B: Casting processesExpendable mold, typically made of sand, plaster, ceramics and similar materials andgenerally are mixed with various binders for improve properties. These materials arerefractories that are capable of withstanding the high temperature of molten metals. Afterthe casting has solidified, the mold is broken up to remove the casting.Permanent mold, normally made of metals that maintain their strength at hightemperatures. They are used repeatedly and are design in such away that the casting canbe removed easily and the mold used for the next casting. Metal molds are betterconductors than expendable mold nonmetallic molds; hence the solidifying casting issubjected to a higher cooling rate which affects the microstructure and grain size of thecasting.Composite molds, which are made of two or more different materials (such as sand,graphite, and metal) combining the advantages of each material. • Fig 11.1(a) shows typical gray-iron castings used in automobiles, including the transmission valve body (left) and the hub rotor with disk-brake cylinder (front), (b) a cast transmission housing, (c) the Polaroid PDC-2000 digital camera with a AZ191D die-cast, high-purity magnesium case and (d) a two-piece Polaroid camera case made by the hot-chamber die-casting process.
2. Sand Casting • Sand casting is still the most prevalent form of casting. • Table 11.2 shows the general characteristics of casting processes. • Basically, sand casting consists of (a) placing a pattern (having the shape of the desired casting) in sand to make an imprint, (b) incorporating a gating system, (c) removing the pattern and filling the mold cavity with molten metal, (d) allowing the metal to cool until it solidifies, (e) breaking away the sand mold, and (f) removing the casting. • Fig 11.2 shows the outline of production steps in a typical sand-casting operation.Sands • Most sand-casting operations use silica sand as mold material. • Sand is inexpensive and is suitable as mold material because of its high- temperature characteristics and high melting point. • There are two general types of sand: naturally bonded (bank sand) and synthetic (lake sand). • Although fine-grained sand enhances mold strength, the fine grains also lower mold permeability (penetrating through pores). • Good permeability of molds and cores allows gases and steam evolved during the casting to escape easily. • Fig 11.2 shows the outline of production steps in a typical sand-casting operation.Types of Sands Molds • Fig 11.3 shows schematic illustration of a sand mold, showing various features. • Sand molds are oven dried (baked) prior to pouring the molten metal; they are stronger than green-sand molds and impart better dimensional accuracy and surface finish to the casting.
3. Patterns • Patterns are used to mold the sand mixture into the shape of the casting and may be made of wood, plastic, or metal. • The selection of a pattern material depends on the size and shape of the casting, the dimensional accuracy and the quantity of castings required, and the molding process. • Fig 11.4 shows a typical metal match-plate pattern used in sand casting. • An important development in molding and pattern making is the application of rapid prototyping. • Fig 11.5 shows the taper on patterns for ease of removal from the sand mold.Cores • For castings with internal cavities or passages, such as those found in an automotive engine block or a valve body, cores are utilized. • Cores are placed in the mold cavity to form the interior surfaces of the casting and are removed from the finished part during shakeout and further processing. • Fig 11.6 shows the examples of sand cores showing core prints and chaplets to support cores.
4. Sand-molding machines • The oldest known method of molding, which is still used for simple castings, is to compact the sand by hand hammering (tamping) or ramming it around the pattern. • Fig 11.7 shows the vertical flaskless molding. (a) Sand is squeezed between two halves of the pattern. (b) Assembled molds pass along an assembly line for pouring. (c) A photograph of a vertical flaskless molding line.The sand-casting operation • After the mold has been shaped and the cores have been placed in position, the two halves (cope and drag) are closed, clamped, and weighted down to prevent the separation of the mold sections under the pressure exerted when the molten metal is poured into the mold cavity. • Fig 11.8 shows schematic illustration of the sequence of operations for sand casting. • Inspection is an important final step and is carried out to ensure that the casting meets all design and quality-control requirements. • Finishing operations may involve machining, straightening, or forging with dies (sizing) to obtain final dimensions.
5. Shell molding • Fig 11.9 shows the shell-molding process, also called the dump-box technique. • The high quality of the finished casting can reduce • cleaning, machining, and other finishing costs significantly. • Complex shapes can be produced with less labor, and the process can be automated fairly easily.
6. Evaporative-pattern casting (lost-foam process) • Evaporative-pattern casting is sometimes referred to as the expendable-pattern casting processes or the expendable mold-expendable pattern processes. • It is unique in that a mold and a pattern must be produced for every casting, whereas the patterns in the processes described thus far are reusable. • The evaporative-pattern casting process uses a polystyrene pattern, which evaporates upon contact with molten metal to form a cavity for the casting; this process is also known as lost-foam casting and falls under the trade name Full- Mold process. • Fig 11.11 shows the schematic illustration of the expendable-pattern casting process, also known as lost-foam or evaporative–pattern casting. • The evaporative-pattern process has a number of advantages over other casting methods: • The process is relatively simple because there are no parting lines, cores, or riser systems. Hence, it has design flexibility. • Inexpensive flasks are satisfactory for the process. • Polystyrene is inexpensive and can be processed easily into patterns having complex shapes, various sizes, and fine surface detail. • The casting requires minimal finishing and cleaning operations.
7. Investment Casting • The investment-casting process, also called the lost-wax process. • Fig 11.3 shows the schematic illustration of the investment casting (lost-wax) process. • Castings produced by this method can be made with very fine detail and from a variety of metals. • Although the mold materials and labor involved make the lost-wax process costly, it is suitable for casting high-melting-point alloys with good surface finishes and close dimensional tolerances; few or no finishing operations, which otherwise would add significantly to the total cost of the casting, are required.
8. Permanent molds • In permanent-mold casting, (also called hard-mold casting), two halves of a mold are made from materials with high resistance to erosion and thermal fatigue, such as cast iron, steel, bronze, graphite, or refractory metal alloys. • The mold cavity and gating system are machined into the mold and, thus, become an integral part of it. • To produce castings with internal cavities, cores made of metal or sand aggregate are placed in the mold prior to casting. • In order to increase the life of permanent molds, the surfaces of the mold cavity usually are coated with a refractory slurry (such as sodium silicate and clay) or sprayed with graphite every few castings. • The molds are clamped together by mechanical means and heated to about 150° to 200°C to facilitate metal flow and reduce thermal damage to the dies due to high- temperature gradients. • Although the permanent-mold casting operation can be performed manually, it can be automated for large production runs. • This process is used mostly for aluminum, magnesium, copper alloys, and gray iron because of their generally lower melting points, although steels also can be cast using graphite or heat-resistant metal molds.Pressure Casting • The molten metal flows into the mold cavity by gravity. In pressure casting (also called pressure pouring or low-pressure casting), the molten metal is forced upward by gas pressure into a graphite or metal mold. • The pressure is maintained until the metal has solidified completely in the mold. • The molten metal also may be forced upward by a vacuum, which also removes dissolved gases and produces a casting with lower porosity.
9. Die Casting• The die casting process is a further example of permanent-mold casting.• Typical parts made by die casting are motor housings, engine blocks, business- machine and appliance components, hand tools, and toys.• In this process, the molten metal is forced into the die cavity at pressures ranging from 0.7 to 700 MPa.• There are two basic types of die-casting machines: hot-chamber and cold- chamber.• Fig 11.18 shows the schematic illustration of the cold-chamber die-casting process.• These machines are large compared to the size of the casting, because high forces are required to keep the two halves of the dies closed under pressure.
10. Process capabilities and machine selection • Die casting has the capability for rapid production of strong, high-quality parts with complex shapes, especially with aluminum, brass, magnesium, and zinc. • Table 11.3 shows the properties and applications of die-casting alloys. • It also produces good dimensional accuracy and surface details, so that parts require little or no subsequent machining or finishing operations (net-shape forming). • Insert molding process is similar to placing wooden sticks in popsicles prior to freezing. • Die-casting dies may be single cavity, multiple cavity (with several identical cavities), combination cavity (with several different cavities), or unit dies (simple small dies that can be combined in two or more units in a master holding die). • Fig 11.19 shows the various types of cavities in a die-casting die.
11. Centrifugal Casting • Centrifugal-casting process utilizes inertial forces (caused by rotation) to distribute the molten metal into the mold cavities. • There are three types of centrifugal casting: true centrifugal casting, semi- centrifugal casting, and centrifuging.True centrifugal casting • In true centrifugal casting, hollow cylindrical parts (such as pipes, gun barrels, bushings, engine-cylinder liners, bearing rings with or without flanges, and streetlamp posts) are produced. • Fig 11.20(a) shows the schematic illustration of the centrifugal-casting process. • Pipes, cylinder liners, and similarly shaped parts can be cast with this process. • Fig 11.20(b) shows the side view of the machine. • Castings with good quality, dimensional accuracy, and external surface detail are produced by this process.Semi-centrifugal casting • An example of semi-centrifugal casting is shown in Fig. 11.21a. • This method is used to cast parts with rotational symmetry, such as a wheel with spokes.
12. Centrifuging • Centrifuging. In centrifuging (also called centrifuge casting), mold cavities of any shape are placed at a certain distance from the axis of rotation. • The molten metal is poured from the center and is forced into the mold by centrifugal forces (Fig. 11.21b). • The properties of the castings can vary by distance from the axis of rotation, as in true centrifugal casting.Squeeze casting • The squeeze casting (or liquid-metal forging) process involves the solidification of molten metal under high pressure. • Fig 11.22 shows the Sequence of operations in the squeeze-casting process. • This process combines the advantages of casting and forging.